# Development of an image-based numerical model for predicting the microstructure–property relationship in alumina trihydrate (ATH) filled poly(methyl methacrylate) (PMMA)

## Abstract

Particulate composites are found in a wide range of applications. Their heterogeneous microstructure affects their bulk behavior and structural performance, however tools for predicting this important structure-property relationship are still lacking. In this study, a numerical method that can provide predictions of the mechanical response of a particulate polymeric matrix composite as a function of volume fraction and particle mean diameter is presented. The work is derived for an alumina trihydrate filled poly(methyl methacrylate) but the methodology is generic and can be used for any particulate composite. Representative Volume elements are determined through images obtained from scanning electron microscopy. The model takes into account the possibility of failure through interface debonding as well as cracks through the matrix. The model predictions for the modulus and fracture strength of the composites are validated through independent experiments on the composite. The numerical results are also used to qualitatively explain the trends measured regarding the fracture toughness of the composites. Compared to other literature on particulate composites, our study is the first to report accurate stress–strain distributions as well as fracture predictions whilst all the necessary model parameters defining the failure criteria are all derived through independent experiments. This paves the way for a relatively simple methodology for determining structure-property relationships in composites design, enabling smarter material utilization and optimal mechanical properties.

## Keywords

Particulate polymeric composites Fracture Micromechanical model Cohesive zone model Brittle matrix cracking Structure–property relationships## 1 Introduction

Particle reinforced polymeric composites appear in a very wide range of applications, e.g. paints, consumer products, automotive parts, explosives and biological systems such as foods. A specific example is the material being investigated in this study, which is alumina trihydrate (ATH) filled poly methyl methacrylate (PMMA) (lightly crosslinked) used in countertop/bench top surfaces with the ATH acting as a flame retardant and smoke suppressant filler to enhance fire safety. At the macro-scale, random arrangements allow such composites to be treated as homogeneous and isotropic. However, at the micro-scale, the heterogeneous structure plays a key role in influencing the mechanical properties of the filled polymers. Understanding how the microstructure impacts the bulk properties is still an active field of research. Specifically, predictive modelling tools for this structure-bulk property relationship are needed such that composite design may be rationalised and made more efficient, replacing costly, trial-and-error experimental approaches.

Well-dispersed non-adhering particles essentially act as a large number of voids and leads to a lower modulus. During the deformation of a polymeric matrix with limited extensibility (e.g. PMMA, which is the matrix used in this study), these voids become cracks and extend to a critical size that causes brittle failure (Lange 1970; Spanoudakis and Young 1984a, b). If particles are well bonded to a brittle matrix, larger strains are required for debonding and the formation of voids (Fu et al. 2008; Hsueh 1989; Young and Beaumont 1977; Zhu et al. 1999). However, research has also indicated that strong adhesion between fillers and matrix may decrease the strength of the resulting composite (Ranade et al. 2006).

For a constant volume fraction, smaller particle size means larger interface, which leads to a higher reinforcement efficiency. However, at high filler volume fractions, the possible agglomeration of smaller particles can lead to non-uniform distributions, and thereby, creating weak regions which cause a decrease in mechanical properties (Dasari et al. 2006; Finnigan 2005).

The effects of the volume fraction on the strength of particle-filled composites have also been investigated (Baptista et al. 2016; Ferreira et al. 1997; Hanumantha-Rao et al. 1998; Wang et al. 2013) with inconclusive results; as the filler content increases, the strength of the composites may increase, decrease or fluctuate. On the other hand, the decrease in particle size can increase the strength as long as the particles are well dispersed (Nakamura et al. 1992; Pukanszky and Vörös 1993; Radford 1971).

At low volume fraction of added particles, a moderate increase in fracture toughness, \(G_{IC} \), can be observed as volume fraction increases (Evans et al. 1985; Hussain et al. 1996; Moloney et al. 1984; Spanoudakis and Young 1984a). At high volume fraction (\(>40\%\)), a further increase in volume fraction could lead to a decrease in \(G_{IC}\) values (Gunel and Basaran 2013b; Stapountzi et al. 2009). This was explained by the fact that the particles tend to agglomerate and cause stress concentrations leading to premature failure (Ferreira et al. 1997). In addition, particle size has been reported to affect the \(G_{IC}\) of composites. However, the trends with particle size vary widely for different materials (Nakamura et al. 1991; Spanoudakis and Young 1984a; Williams 2010). For example, when the particle radius exceeded 10 \(\upmu \hbox {m}\), the addition of larger silica particles in epoxy matrix led to a higher \(G_{IC}\) (Nakamura et al. 1991) while increasing particle radius in the case of glass particles led to a decrease in \(G_{IC}\) for the same matrix (Spanoudakis and Young 1984a).

In an effort to explain such contradictory experimental observations, a number of modelling studies have been reported. Historically, these are based on analytical models for predicting the deformation properties (e.g. modulus) of the composites. The models are based on the description of the strain field inside and around a rigid particle embedded in an infinite matrix (Eshelby 1957; Hashin and Shtrikman 1963; Mori and Tanaka 1973; Teng 2010) as derived by Eshelby (1957) for linear elasticity. Eshelby’s work provided the basis for several micromechanical models that followed, resulting in the well-known Mori and Tanaka method (Mori and Tanaka 1973), several bounding methods such as the Hashin and Shtrikman (1963), Weng (1992) and Lielens et al. (1998). For a comprehensive review of such models the reader is referred to Stapountzi et al. (2009).

Taking the imperfect interface into consideration, Teng (2010) developed a three-phase model derived from the Mori–Tanaka solution whereas Benveniste (1987) and Nie and Basaran (2005) have used spring elements to model this imperfect interface. Williams (2010) derived an analytical model for the prediction of the debonding process in a particle filled composite based on a unit cell. More recently, Jiang (2016) reviewed several analytical micro-mechanics-based models and proposed a model taking into account matrix cracking and debonding, the latter through a Weibull distribution function for the cumulative probability of particle debonding.

Several studies have used the cohesive zone approach (Xu and Needleman 1993) to model the filler/matrix interfacial behaviour. The latter has been largely facilitated through the large increase in available computational power. Hashemi et al. (2015) used a potential based cohesive model to characterize interfacial debonding in composite materials containing multi-coated particles. Ponnusami et al. (2015) studied the interaction between an approaching crack and a particle as a function of the mismatch in elastic and fracture properties. Cohesive zone models have also been used in the metal matrix composite (MMC) community; for example Charles et al. (2010) studied the competition between interface debonding and particle fracture whereas Qing (2014) studied the influence of particle arrangement and interface strength on the mechanical behaviour of MMCs. Using a multi-particle unit cell model, Basaran and Gunel (2013) and Gunel and Basaran (2013b) studied the influence of interphase properties and interparticle distance on large deformation micromechanics of PMMA/ATH composites. However, the assumptions of the fillers being perfect spheres and equally spaced in all directions, limit the application of this approach to real composites (Tarleton et al. 2013). The majority of the numerical modelling studies have used simulated microstructures or ideal, regular unit cell geometries. However, another implication of the advancement in finite element model simulations and computational power is that real microstructures as measured from microscopic studies may be used instead (Arora et al. 2015; Dastgerdi et al. 2016; Mcwilliams et al. 2013). These lead to more accurate predictions of the mechanical properties (Tarleton et al. 2013).

Though an immense amount of work, as summarised above, is reported in the literature on structure–property relationships for particulate composites, there is still a lack of relatively simple and cost-efficient predictive micromechanical models that can deliver predictions for the mechanical response and in particular the fracture properties of these materials. This work sets out a methodology to achieve this aim. Numerical simulations from previous studies (e.g. Arora et al. 2015; Basaran and Gunel 2013; Gunel and Basaran 2013a) only accounted for composite failure by interface debonding. In this work and for the first time, composite failure by both interface debonding and matrix cracking was incorporated. A real microstructure-based FEA approach for predicting the mechanical behaviour and fracture patterns in ATH filled PMMA composites is presented. The usage of real scanning electron microscopy (SEM) microstructural images in defining the representative volume elements (RVEs) for the modelling study, enables the simulation of agglomeration-induced stress concentrations. The numerical predictions are compared and validated against experimental data measured in this study. Most importantly, the common problem regarding the difficulty of experimental calibration of the associated damage models is addressed through direct experimental identification. The suggested methodology is relatively simple and generic such that it could form a powerful design tool in particulate composite design.

## 2 Materials and experimental methods

Particle size and volume fraction of the ATH/PMMA composites (Dupont 2014)

Material code | Volume fraction ATH filler (%) | Mean particle size of ATH filler (\(\upmu \hbox {m}\)) |
---|---|---|

A | 34.7 | 15 |

B | 39.4 | 8 |

C | 39.4 | 15 |

D | 39.4 | 25 |

E | 44.4 | 15 |

Tensile tests were performed on unfilled PMMA for determining its elastic modulus and fracture strength. Type M-I (ASTM 1998) ‘bone-shaped’ tensile specimens were provided by the material supplier. The width, gauge length and thickness of each specimen were 10, 50 and 10 mm, respectively. An Instron 3369 system with a 5 kN load cell was used for conducting the tests. The crosshead motion rate was set at 5 mm/min.

Flexural tests and single edge notched bending (SENB) tests were performed to investigate the mechanical properties of the composites. Both tests were performed using an Instron 4466 system (5 kN load cell) and the deflection was measured using digital image correlation (DIC) software DaVis (LaVision 2006). The flexural tests were performed according to ASTM D790M-10 standard (ASTM 2010). The length, width and thickness of the rectangular specimens were 125, 10 and 6 mm, respectively. The loading span was set as 96 mm, while the crosshead motion rate was 2.1 mm/min. The tests were performed up to failure to determine the strength of the composites.

The SENB tests were performed according to ISO 13586 (ISO 2000) on both the composites and unfilled PMMA using the Instron 4466 system with a 5 kN load cell. The dimensions of the SENB specimens were \(50\times 10\times 5\) (mm\(^{3}\)), where 5 mm was the thickness of the samples. A notch of 5 mm in length was cut along the centre of each specimen using a horizontal milling machine. In addition, to avoid the overestimation of the fracture toughness, the tip of each notch was tapped using a new liquid-nitrogen-cooled razor blade to introduce a sharp crack. The loading span was set at 40 mm. The tests were performed at a cross-head motion rate of 1 mm/min, whilst the compliance correction test was performed at 0.1 mm/min.

A Hitachi S-3400N scanning electron microscope was used to observe the fracture surfaces near the crack tips of the tested SENB samples. The images were captured using the back scattered electrons (BSE) mode. In addition, fifteen images of the polished surface of each composite were taken using the secondary electron (SE) mode and were processed using ImageJ (Rasband 2016) in order to define the RVEs employed in the numerical simulations (see Sect. 3).

In addition to the experiments outlined above, compact tension tests were also performed in order to characterise the properties of the interface between the ATH particle and the PMMA matrix in accordance of the method proposed by Tan et al. (2005b). Since the same coupling agent was used in all the composites, CT tests were only performed on three replicates of composite C. The tests were performed according to the ISO 13586 standard (ISO 2000) on an Instron 3369 system fitted with a 5 kN load cell, at a crosshead motion rate of 10 mm/min. To ensure the crack propagated along the centre line of each specimen, a shallow side groove (radius \(\approx 1\,\hbox {mm}\)) was machined on the back surface of the sample; the front surface was left flat so that DIC could be performed. DIC was performed on the images captured using a \(\hbox {Phantom}^\circledR \) Miro M/R/LC310 high speed camera at 500 frames per second in order to obtain the strain field around the crack tip. The size of the field of view was 22.4 mm \(\times \) 20 mm and the resolution was 448 pixels by 400 pixels. Therefore, the resolution of the images was \(0.05 \times 0.05\,\hbox {mm}^{2}/\hbox {pixel}\). According to Vendroux and Knauss (1998), the DIC technique can measure the displacement in the order of 0.005 pixel, which was about 0.25 \(\upmu \hbox {m}\) in the present work.

## 3 Numerical model details

In order to derive predictions of the modulus and strength of the composite as a function of its microstructure, numerical simulations were performed using RVEs derived from the SEM micrographs of the polished composite surfaces. The commercial finite element analysis software Abaqus with the explicit solver (Dassault 2016a) was used for all analyses.

### 3.1 Model geometry and boundary conditions

Due to the difficulty of generation and the associated high computational cost of 3D FE geometries, 2D plane strain geometries were used in this study. The usage of the 2D geometries was also justified by its proven satisfactory accuracy (Arora et al. 2015) and the low aspect ratio of the fillers (approximately 1.2, see Sect. 4.2).

Using image processing and reconstruction algorithms developed by Tarleton et al. (2012), the SEM images of the polished composite surfaces were converted into 2D geometries. Once a particle was approximated as a polygon, the particle/matrix interfacial region is produced by offsetting the boundary a small distance inwards. The interfacial region is then assigned as a single layer of cohesive elements.

A typical example of the SEM image conversion to the RVE modelled in FEA is shown in Fig. 2. For each composite, fifteen SEM images taken from random positions on the sample were reconstructed into RVEs. The reconstructed 2-dimensional RVEs were rectangular. Three different RVE sizes, i.e. horizontal \(\times \) vertical: \(120 \, \upmu \hbox {m} \times 90 \,\upmu \hbox {m},\, 200 \, \upmu \hbox {m} \times 150 \, \upmu \hbox {m}\) and \(300 \, \upmu \hbox {m} \times 225 \, \upmu \hbox {m}\), were compared for studying the effect of the RVE size on the predictions. In addition, the mesh dependence of the FE prediction was investigated by using three different mesh sizes (0.75, 1.5 and 3 \(\upmu \hbox {m}\)). For the FE prediction to be comparable with the experimental results, plane strain was assumed. Therefore, the matrix and filler were meshed using 4-node bilinear elements CPE4R (reduced integration with hourglass control), whilst the interface was meshed using cohesive elements COH2D4.

A simple uniaxial tensile deformation was applied as the boundary condition despite flexural tests being performed to experimentally investigate the modulus and strength of the ATH/PMMA composites. During bending of a sample, zero stress prevails at the neutral axis whereas tensile and compressive stresses build up at either side of the neutral axis. Once the material fails, the corresponding load is taken for calculation of the flexural strength. Since the material fails in the portion under tension, the flexural strength should be theoretically the same as the tensile strength. However, in reality there are defects present in the specimens. In the tensile test, the defects affect the strength uniformly, whilst in flexure, defects near the top or the bottom surfaces will have a larger effect than the same type of defects located near or on the neutral axis. Therefore, the value of the flexural strength is approximately 1.5–2.1 times higher than that of the tensile strength (Sahagian and Proussevitch 1998). The effects of the defects are not simulated directly in the FE simulation, which means the strength prediction obtained using tensile and flexural boundary conditions would be the same. Therefore, a tensile boundary condition in the form of a 5% deformation on the top surface was applied to each RVE in the vertical direction (Fig. 2). The bottom surface was constrained in the vertical direction with one node on the bottom left corner constrained in both directions. The two side edges were left free which according to Arora et al. 2015) gives results which are as accurate as periodic boundary conditions. Also it is worth noting that periodic boundary conditions are applicable for repeatable RVEs, while the present RVEs of the composites are random and not repeatable.

### 3.2 Damage models and material definition

Both the constituents were treated as linear elastic isotropic materials. Note that the structure of ATH particles is graphitic in nature, so modelling the correct anisotropy would increase the complexity significantly. In addition, the orientation of the graphitic planes of each particle embedded in the composite is unknown and modelling such effects would be computationally prohibitive. It is therefore assumed here that failure in the composites is primarily due to interface debonding and matrix cracking; this led to the simplifying assumption that the filler is an isotropic, elastic material with no need to model inter-particle fracture. The elastic properties of the matrix and filler were taken from the experiments described in Sect. 2 or from literature (also summarised later in Table 3).

Debonding along the filler/matrix interface is one of the main failure mechanisms of composites. A bilinear traction separation law was used for simulating the interfacial debonding through the cohesive elements placed along the boundaries of the particles (Dassault-Systèmes 2016b). After the onset of damage, the cohesive elements soften and fail, at which point their stiffness is degraded to zero. The determination of the interfacial properties, i.e. interfacial linear stiffness, interfacial cohesive strength and interfacial cohesive fracture energy are presented in Sect. 4.5. The same cohesive zone properties were assumed for mode I and mode II whereas the mixed mode failure locus was taken to be linear.

In addition to the debonding failure mode at the particle-matrix interface, the numerical simulations accounted for possible fracture propagating in the matrix. PMMA fails by crazing (Döll 1983; Saad-Gouider et al. 2006) and its failure mechanism can be determined from inverse analysis (Elices et al. 2002) or crack tip field analysis (Réthoré and Estevez 2013). However, a brittle cracking model was used for simulating this matrix failure in the current study. This is mainly because in particle-filled composites, the toughening effects of the fillers prevent crazing of the polymer matrix (Chee et al. 2012). Meanwhile, as shown by Nie et al. (2006), the failure of ATH/PMMA composites is initiated by the debonding between filler/matrix and the damage of the PMMA matrix is caused by the growth of the cavity, which happens so fast that crazing cannot be observed. In addition, to simulate the crazing of PMMA, cohesive elements need to be used over the entire RVE (Tijssens et al. 2000), which may complicate the model significantly and increase the computational cost. Therefore, in this study, crack initiation is detected using a simple Rankine criterion, which means that a crack is formed when the principal tensile stress reaches the crack initiation stress of the brittle material. Once the criterion has been met, a first crack is assumed to have formed. The crack growth direction is controlled using a fixed, orthogonal model, which means the crack grows in a direction normal to the direction of maximum tensile principal stress at the time of crack initiation. Little experimental data of the crack initiation stress of PMMA is available. Therefore, a theoretical value, \(E_m /10\), is first assumed. However, this value is related to the cohesive forces between atoms (Lawn 1993), which means that for brittle solid such as the PMMA matrix studied here, the value \(E_m /10\) may lead to overestimation of the composite strength. Therefore, lower values of the crack initiation stress, i.e. \(E_m /20, E_m /30{\ldots }\), are also used in a parametric study in order to investigate the influence of this value on the model’s predictions. Note that these values will be later compared to the failure strength of PMMA.

*p*and \(e_{max}^{cr} \) are material parameters.

For simplicity the value of *p* was chosen as 1, whereas \(e_{max}^{cr} \) was set to 1%. The latter is the typical failure strain of PMMA (Kaplan 1999).

## 4 Experimental results

### 4.1 Experimental results for PMMA matrix

The modulus and strength of unfilled PMMA matrix is measured as \(3.02\pm 0.03 \, \hbox {GPa}\) and \(76\pm 3\, \hbox {MPa}\), respectively. The fracture energy of unfilled PMMA obtained using SENB tests is \(395.1\pm 27.1 \, \hbox {N/m}\). The results agree with reported data in literature (Kaplan 1999) and were used as input in the numerical simulations.

### 4.2 SEM microstructures of composites

### 4.3 Composite flexural test results

Modulus and strength of the ATH/PMMA composites obtained using flexural tests

Composite | A | B | C | D | E |
---|---|---|---|---|---|

Volume fraction (%) | \(35\pm 2\) | \(39\pm 2\) | \(40\pm 3\) | \(39\pm 2\) | \(44\pm 2\) |

Particle Diameter D[4,3] (\(\upmu \hbox {m}\)) | 15.1 | 9.3 | 15.1 | 23.0 | 15.1 |

Modulus (GPa) | \(7.3\pm 0.3\) | \(7.5\pm 0.5\) | \(7.6\pm 0.2\) | \(7.8 \pm 0.1\) | \(8.8 \pm 0.1\) |

Strength (MPa) | \(75.4\pm 3.0\) | \(82.4\pm 5.3\) | \(69.1\pm 5.2\) | \(66.4\pm 3.5\) | \(70.8\pm 4.5\) |

In Table 2, the flexural strength of the composites is shown to initially decrease as the filler loading increases (composites A, C and E). The decrease is less than 8%, which is not statistically high enough to point to an effect of filler volume fraction on strength. This may be caused by the balance between the strengthening effect of the rigid particles acting as barriers to crack growth and the weakening effect of particle agglomerations.

### 4.4 Fracture toughness of the composites

Figure 5 shows the effect of filler content on the values of \(K_{IC} \) and \(G_{IC}\) of ATH/PMMA composites. It can be seen that the value of \(G_{IC}\) decreased as the volume fraction increased, while the value of \(K_{IC}\) remained constant. The addition of rigid particles may cause an increase in \(K_{IC}\) values of polymers, because as the particles are pinned in the matrix, higher loads are required for the cracks to grow within the material. However, due to the high filler content used in this work, an increase in the volume fraction can cause particle agglomeration and hence, induce stress concentrations, which can initiate and extend cracks until the critical crack size is reached and the material fails. Therefore, the balance between the toughening effects of the rigid particles and the weakening effects of the particle agglomeration could be the main reason of the constant \(K_{IC} \) values as the filler content varies.

The effect of particle diameter on \(K_{IC} \) and \(G_{IC} \) values of ATH/PMMA composites is shown in Fig. 6. With increasing particle diameter, both \(K_{IC} \) and \(G_{IC} \) values display increasing trends. It is suggested here that this phenomenon is due to the higher probability of particle agglomeration taking place for the smaller particles at the high volume fractions studied hence leading to lower \(K_{IC} \) and \(G_{IC} \) values.

### 4.5 Experimental determination of interfacial properties for the CZM law

Figure 9 shows the horizontal (*u*-), vertical (*v*-) and normal strain perpendicular to the fracture plane (\(\varepsilon _{yy} )\) measured using DIC with the raw image as the background at the point of crack initiation. From the macroscopic strain field around the crack tip (see Fig. 9c), the macroscopic cohesive law of the ATH/PMMA composite (Fig. 10) was obtained by plotting the cohesive stress (i.e. the value of \(E_c \varepsilon _{yy} \) as close to the crack tip as possible, see position indicated by a red ‘X’ mark in Fig. 9) against the crack opening width (i.e. the difference between the *v*- displacements just above and under the fracture plane at the crack tip). As shown in Fig. 10, the macroscopic cohesive strength is 54.5 MPa, whilst the critical crack opening width is 0.015 mm. These values give a macroscopic cohesive energy of \(\sim \) 410 N/m which agrees with the fracture energy of composite C obtained using SENB tests (\(\sim \) 400 N/m, see Fig. 5b).

A summary of the material properties used as input in the numerical simulations

Materials | Property | Value | Source |
---|---|---|---|

PMMA | Elastic modulus (GPa), \(E_m \) | 3.02 | Tensile test |

Poisson’s ratio, \(v_m \) | 0.38 | Jung et al. (2000) | |

Fracture toughness (N/m), \(G_{ICm} \) | 395.1 | SENB test | |

Crack initiation stress (GPa) | \(E_m /10,\quad E_m /20,\quad E_m /30\) | ||

ATH | Elastic modulus (GPa), \(E_f \) | 76 | Jung et al. (2000) |

Poisson’s ratio, \(v_f \) | 0.24 | Jung et al. (2000) | |

ATH/PMMA interface | Interfacial linear modulus (GPa/\(\upmu \hbox {m}\)), \(k_\sigma \) | 3.61 | CT test and DIC |

Interfacial cohesive strength (MPa), \(\sigma _{max}^{int} \) | 119 | CT test and DIC | |

Interfacial cohesive energy (N/m), \(\gamma _{int} \) | 430 | CT test and DIC |

*A*is the area of the crack surface. The value of \(U_{coh} \) is found from the area under the cohesive law shown in Fig. 10. It can also be expressed as:

## 5 Results from the numerical simulations

This section presents the results from the numerical simulations of the RVEs being subjected to tensile deformations. The predictions are compared to the experimentally derived values of modulus and fracture strength as a function of volume fraction and particle size. The material property parameters used in the simulations are summarised in Table 3.

### 5.1 Effect of the RVE size

The model predictions obtained corresponding to the three RVE sizes showed that the modulus and strength were in agreement (within 6 and 3% respectively). Despite a small effect on the global load-displacement response, the change in RVE size was found to affect the crack path (see Fig. 12). The application of a bigger RVE size may provide a crack path in higher compliance with the actual situation. Therefore, the RVE size of \(200 \,\upmu \hbox {m} \times 120\,\upmu \hbox {m}\) was selected for further study.

### 5.2 Mesh dependence study

Figure 13 shows the effect of the mesh density on the stress–strain curves obtained using the FE simulation. The numerically predicted values for elastic modulus and fracture strength are not affected by the mesh size. However, it is shown that the mesh density affects the post-crack behaviour of the composite. This indicates a mesh dependency of the post-crack FE prediction, however it is small. The mesh dependency was also observed in the predicted crack path (see Fig. 14). In a more finely meshed RVE, micro-cracks existed besides the main crack, which could be more realistic (Tarleton et al. 2012). Therefore, despite the higher computational cost, a finer mesh (\(\hbox {mesh size }= 0.75 \, \upmu \hbox {m}\)) was selected for subsequent investigations.

### 5.3 Elastic modulus of the composites

As a validation of the microstructural image based modelling technique, the elastic modulus obtained from the FE models and the experiments are compared. The results are also compared to the micromechanical model by Lielens for extra verification (Lielens et al. 1998).

The micromechanical Lielens model (Lielens et al. 1998) was next employed to provide a comparison with the experimental and numerical predictions. The numerical predictions for the composite’s modulus are plotted against the actual RVE volume fraction and compared with the Lielens predictions in Fig. 16 as well as with the experimental data. It is now observed that the numerical and analytical Lielens predictions are both very close to the experimental data. The omission of the finer particles in the models is not thought to be adversely affecting the accuracy of the predictions for fracture strength as debonding of the larger particles occurs first and therefore limits critically the composite’s strength (Jung et al. 2000).

### 5.4 Elastic strength and fracture toughness of the composites

From the output stress contours shown in Fig. 18, the stress inside the particles was found to be higher than the stress distributed in the matrix. In addition, the bigger the particle, the higher the stress the particle is bearing. Therefore, the failure of the composites generally starts with the debonding of the relatively big particles, which may also be observed more clearly when the stress degradation factor (SDEG)contours are plotted in Fig. 19; SDEG values of 1 signify fully debonded regions (red contour) and values of SDEG \(=\) 0 show undamaged surfaces (blue contours). Therefore, the small effect of the volume fraction on the elastic strength shown in Fig. 17a can be explained by the similar particle size distribution in composites A, C and E (see Fig. 1). It is also worth noting here that even though the stress in the particles is higher than the matrix, its magnitude is only about 300 MPa. This is smaller than the typical strength of engineering ceramics. Therefore, the assumption that there is no failure in the particles is in fact justified by the numerical results.

Finally, determining a methodology such that the values of \(K_{IC} \) and \(G_{IC} \) can also be predicted through the numerical method, in addition to the modulus and strength of the composite, is a current aim and work is underway towards achieving this.

## 6 Conclusions

A combined experimental-numerical study was conducted in order to highlight the effect of the microstructure on the global response of ATH/PMMA particulate composites. The interface behaviour is characterised via a cohesive traction-separation model while the damage of the matrix is defined using a brittle cracking model. The parameters used in the FE simulation were obtained through appropriate experiments. The comparison between the experimental results and FE predictions indicates that the SEM image-converted RVE FE model can provide accurate predictions of the elastic modulus as well as the failure strength of particle filled composite. For the failure strength, the numerical trends with particle diameter and volume fraction were extremely close to the trends observed experimentally, giving confidence in the developed models. The fracture strength of the composites increased with decreasing particle size. This was caused by the more uniformly distributed stress due to the narrower particle size distribution of the composites filled with smaller particles. In addition, the effect of filler content on the composite strength is insignificant due to the similar filler size distribution. For the fracture toughness, it was shown that increasing particle size led to higher \(K_{IC} \) and \(G_{IC} \) values due to the blocking/deflecting effect of the bigger particles. Furthermore, according to the strain map obtained from the SEM image-converted geometry, the FE predictions indicate a higher likelihood of agglomeration-induced cracks initiating in the matrix in the composites with a smaller mean particle diameter. On the other hand, as the volume fraction increased, the \(G_{IC} \) values decreased due to the restraining effects of the rigid particles on the matrix deformation, but the \(K_{IC} \) values showed little change due to the balance between the toughening effect of the rigid particles and the weakening effect of particle agglomeration.

The methodology presented here can be applied to any particulate composite. The important results highlighted above were enabled due to the novelty of our method over related studies reported in the literature. Specifically the main advantages are: (i) the complex real microstructure of the composite is taken into account, (ii) both matrix and interface fracture mechanisms are addressed, and (iii) all the parameters needed as inputs for the simulation of matrix and interface damage are extracted from independent experiments (they are not fitted parameters). The accuracy of the model in predicting accurate trends with both volume fraction and particle mean diameter was remarkable (within 4% for fracture stress) and therefore it forms a significant step towards the design of particulate composites. The developed models lend themselves for parametric studies to readily and cost-efficiently quantify the effect of various quantities related to the material (e.g. interface strength) or microstructural features (e.g. particle size) so as to inform the material designer on how to tune the various parameters to meet the demands of a specific application.

## Notes

### Acknowledgements

The authors would like to thank E.I. DuPont de Nemours and Company, USA, for supplying the composite materials of the study.

## References

- Arora H, Tarleton E, Li-Mayer J, Charalambides M, Lewis D (2015) Modelling the damage and deformation process in a plastic bonded explosive microstructure under tension using the finite element method. Comput Mater Sci 110:91–101CrossRefGoogle Scholar
- ASTM (1998) D638M-84, standard test method for tensile properties of plastics. American Society for Testing and Materials, West ConshohockenGoogle Scholar
- ASTM (2010) D790M-10, standard test methods for flexural properties of unreinforced and reinforced plastics and electrical insulating materials. American Society for Testing and Materials, West ConshohockenGoogle Scholar
- Baptista R, Mendão A, Guedes M, Marat-Mendes R (2016) An experimental study on mechanical properties of epoxy-matrix composites containing graphite filler. Procedia Struct Integr 1:74–81CrossRefGoogle Scholar
- Basaran C, Gunel E (2013) Predicting elastic modulus of particle filled composites. Int J Mater Struct Integr 7:100–108CrossRefGoogle Scholar
- Benveniste Y (1987) A new approach to the application of Mori–Tanaka’s theory in composite materials. Mech Mater 6:147–157CrossRefGoogle Scholar
- Charles Y, Estevez R, Bréchet Y, Maire E (2010) Modelling the competition between interface debonding and particle fracture using a plastic strain dependent cohesive zone. Eng Fract Mech 77:705–718CrossRefGoogle Scholar
- Chee CY, Song N, Abdullah LC, Choong TS, Ibrahim A, Chantara T (2012) Characterization of mechanical properties: low-density polyethylene nanocomposite using nanoalumina particle as filler. J Nanomater 2012:118CrossRefGoogle Scholar
- Döll W (1983) Optical interference measurements and fracture mechanics analysis of crack tip craze zones. In: Kausch HH (ed) Crazing in polymers. Springer, Berlin, pp 105–168. https://doi.org/10.1007/BFb0024057 CrossRefGoogle Scholar
- Döll W, Könczöl L (1990) Micromechanics of fracture under static and fatigue loading: optical interferometry of crack tip craze zones. In: Kaush HH (ed) Crazing in polymers, vol 2. Springer, Berlin, pp 137–214CrossRefGoogle Scholar
- Dasari A, Yu Z-Z, Yang M, Zhang Q-X, Xie X-L, Mai Y-W (2006) Micro-and nano-scale deformation behavior of nylon 66-based binary and ternary nanocomposites. Compos Sci Technol 66:3097–3114CrossRefGoogle Scholar
- Dassault-Systèmes (2016a) Abaqus 6.14, Dassault Systèmes, Vélizy-Villacoublay, FranceGoogle Scholar
- Dassault-Systèmes (2016b) Cohesive elements. Dassault Systèmes, Vélizy-Villacoublay, FranceGoogle Scholar
- Dassault-Systèmes (2016c) A cracking model for concrete and other brittle materials, 4.5.3. Abaqus 6.14 edn. Dassault Systèmes, Vélizy-Villacoublay, FranceGoogle Scholar
- Dastgerdi JN, Marquis G, Anbarlooie B, Sankaranarayanan S, Gupta M (2016) Microstructure-sensitive investigation on the plastic deformation and damage initiation of amorphous particles reinforced composites. Compos Struct 142:130–139CrossRefGoogle Scholar
- Dupont (2014) E.I. DuPont Nemours & Co. (Inc.), Safety data sheetGoogle Scholar
- Elices M, Guinea G, Gomez J, Planas J (2002) The cohesive zone model: advantages, limitations and challenges. Eng Fract Mech 69:137–163CrossRefGoogle Scholar
- Eshelby JD (1957) The determination of the elastic field of an ellipsoidal inclusion, and related problems. Proc R Soc Lond A Math Phys Eng Sci 241:376–396. https://doi.org/10.1098/rspa.1957.0133 CrossRefGoogle Scholar
- Evans A, Williams S, Beaumont P (1985) On the toughness of particulate filled polymers. J Mater Sci 20:3668–3674CrossRefGoogle Scholar
- Ferreira JM, Costa JD, Capela C (1997) Fracture assessment of PMMA/Si kitchen sinks made from acrylic casting dispersion. Theor Appl Fract Mech 26:105–116CrossRefGoogle Scholar
- Finnigan B et al (2005) Segmented polyurethane nanocomposites: impact of controlled particle size nanofillers on the morphological response to uniaxial deformation. Macromolecules 38:7386–7396CrossRefGoogle Scholar
- Fu S-Y, Feng X-Q, Lauke B, Mai Y-W (2008) Effects of particle size, particle/matrix interface adhesion and particle loading on mechanical properties of particulate-polymer composites. Compos B Eng 39:933–961CrossRefGoogle Scholar
- Gunel E, Basaran C (2013a) Influence of filler content and interphase properties on large deformation micromechanics of particle filled acrylics. Mech Mater 57:134–146CrossRefGoogle Scholar
- Gunel E, Basaran C (2013b) Influence of volume fraction and interphase properties on large deformation micromechanics of particle filled acrylics. Mech Mater 57:134–146CrossRefGoogle Scholar
- Hanumantha-Rao K, Forssberg KSE, Forsling W (1998) Interfacial interactions and mechanical properties of mineral filled polymer composites: wollastonite in PMMA polymer matrix. Colloids Surf A Physicochem Eng Asp 133:107–117CrossRefGoogle Scholar
- Hashemi R, Spring DW, Paulino GH (2015) On small deformation interfacial debonding in composite materials containing multi-coated particles. J Compos Mater 49:3439–3455CrossRefGoogle Scholar
- Hashin Z, Shtrikman S (1963) A variational approach to the theory of the elastic behaviour of multiphase materials. J Mech Phys Solids 11:127–140CrossRefGoogle Scholar
- Hsueh CH (1989) Effects of aspect ratios of ellipsoidal inclusions on elastic stress transfer of ceramic composites. J Am Ceram Soc 72:344–347CrossRefGoogle Scholar
- Hussain M, Nakahira A, Nishijima S, Niihara K (1996) Fracture behavior and fracture toughness of particulate filled epoxy composites. Mater Lett 27:21–25CrossRefGoogle Scholar
- ISO (2000) 13586-2000, Plastics—determination of fracture toughness (KIC and GIC)—linear elastic fracture mechanics (LEFM) approach. International Organization for Standardization, GenevaGoogle Scholar
- Jiang Y (2016) An analytical model for particulate reinforced composites (PRCs) taking account of particle debonding and matrix cracking. Mater Res Express 3:106501CrossRefGoogle Scholar
- Jung G-D, Youn S-K, Kim B-K (2000) Development of a three-dimensional nonlinear viscoelastic constitutive model of solid propellant. J Braz Soc Mech Sci 22:457–476CrossRefGoogle Scholar
- Kaplan WA (1999) Modern plastics encyclopedia’99. Mc Graw-Hill/Le Quinio, New YorkGoogle Scholar
- Lange F (1970) The interaction of a crack front with a second-phase dispersion. Philos Mag 22:0983–0992CrossRefGoogle Scholar
- LaVision (2006) DaVis 7.2th. LaVision Inc, GoettingenGoogle Scholar
- Lawn B (1993) Fracture of brittle solids. Cambridge University Press, CambridgeCrossRefGoogle Scholar
- Lielens G, Pirotte P, Couniot A, Dupret F, Keunings R (1998) Prediction of thermo-mechanical properties for compression moulded composites. Compos A Appl Sci Manuf 29:63–70CrossRefGoogle Scholar
- Mcwilliams B, Sano T, Yu J, Gordon A, Yen C (2013) Influence of hot rolling on the deformation behavior of particle reinforced aluminum metal matrix composite. Mater Sci Eng A 577:54–63CrossRefGoogle Scholar
- Moloney AC, Kausch HH, Stieger HR (1984) The fracture of particulate-filled epoxide resins. J Mater Sci 19:1125–1130. https://doi.org/10.1007/bf01120021 CrossRefGoogle Scholar
- Mori T, Tanaka K (1973) Average stress in matrix and average elastic energy of materials with misfitting inclusions. Acta Metall 21:571–574CrossRefGoogle Scholar
- Nakamura Y, Yamaguchi M, Kitayama A, Okubo M, Matsumoto T (1991) Effect of particle size on fracture toughness of epoxy resin filled with angular-shaped silica. Polymer 32:2221–2229CrossRefGoogle Scholar
- Nakamura Y, Yamaguchi M, Okubo M, Matsumoto T (1992) Effect of particle size on mechanical properties of epoxy resin filled with angular-shaped silica. J Appl Polym Sci 44:151–158CrossRefGoogle Scholar
- Nie S, Basaran C (2005) A micromechanical model for effective elastic properties of particulate composites with imperfect interfacial bonds. Int J Solids Struct 42:4179–4191CrossRefGoogle Scholar
- Nie S, Basaran C, Hutchins CS, Ergun H (2006) Failure mechanisms in PMMA/ATH acrylic casting dispersion. J Mech Behav Mater 17:79–96CrossRefGoogle Scholar
- Ponnusami SA, Turteltaub S, van der Zwaag S (2015) Cohesive-zone modelling of crack nucleation and propagation in particulate composites. Eng Fract Mech 149:170–190CrossRefGoogle Scholar
- Pukanszky B, Vörös G (1993) Mechanism of interfacial interactions in particulate filled composites. Compos Interfaces 1:411–427Google Scholar
- Qing H (2014) Micromechanical study of influence of interface strength on mechanical properties of metal matrix composites under uniaxial and biaxial tensile loadings. Comput Mater Sci 89:102–113CrossRefGoogle Scholar
- Réthoré J, Estevez R (2013) Identification of a cohesive zone model from digital images at the micron-scale. J Mech Phys Solids 61:1407–1420CrossRefGoogle Scholar
- Radford K (1971) The mechanical properties of an epoxy resin with a second phase dispersion. J Mater Sci 6:1286–1291CrossRefGoogle Scholar
- Ranade RA, Ding J, Wunder SL, Baran GR (2006) UHMWPE as interface toughening agent in glass particle filled composites. Compos A Appl Sci Manuf 37:2017–2028CrossRefGoogle Scholar
- Rasband WS (2016) ImageJ 1.5.0, National Institutes of Health, Bethesda, Maryland, USA. http://imagej.nih.gov/ij/
- Roux S, Hild F (2006) Stress intensity factor measurements from digital image correlation: post-processing and integrated approaches. Int J Fract 140:141–157CrossRefGoogle Scholar
- Saad-Gouider N, Estevez R, Olagnon C, Seguela R (2006) Calibration of a viscoplastic cohesive zone for crazing in PMMA. Eng Fract Mech 73:2503–2522CrossRefGoogle Scholar
- Sahagian DL, Proussevitch AA (1998) 3D particle size distributions from 2D observations: stereology for natural applications. J Volcanol Geotherm Res 84:173–196CrossRefGoogle Scholar
- Spanoudakis J, Young R (1984a) Crack propagation in a glass particle-filled epoxy resin, part I. J Mater Sci 19:473–486CrossRefGoogle Scholar
- Spanoudakis J, Young RJ (1984b) Crack propagation in a glass particle-filled epoxy resin, part II. J Mater Sci 19:487–496. https://doi.org/10.1007/bf02403235 CrossRefGoogle Scholar
- Stapountzi OA, Charalambides MN, Williams JG (2009) Micromechanical models for stiffness prediction of alumina trihydrate (ATH) reinforced poly(methyl methacrylate) (PMMA): effect of filler volume fraction and temperature. Compos Sci Technol 69:2015–2023CrossRefGoogle Scholar
- Stapountzi OA, Charalambides MN, Williams JG (2011) The fracture toughness of a highly filled polymer composite. In: Kounadis AN, Gdoutos EE (eds) Recent advances in mechanics: selected papers from the symposium on recent advances in mechanics. Academy of Athens, Athens, Greece, 17–19 September, 2009, Organised by the Pericles S. Theocaris Foundation in Honour of P.S. Theocaris, on the tenth anniversary of his death. Springer, Dordrecht, pp 447–459. https://doi.org/10.1007/978-94-007-0557-9_24
- Tan H, Huang Y, Liu C, Geubelle P (2005a) The Mori–Tanaka method for composite materials with nonlinear interface debonding. Int J Plast 21:1890–1918CrossRefGoogle Scholar
- Tan H, Liu C, Huang Y, Geubelle P (2005b) The cohesive law for the particle/matrix interfaces in high explosives. J Mech Phys Solids 53:1892–1917CrossRefGoogle Scholar
- Tarleton E, Charalambides M, Leppard C (2012) Image-based modelling of binary composites. Comput Mater Sci 64:183–186CrossRefGoogle Scholar
- Tarleton E, Charalambides M, Leppard C, Yeoh J (2013) Micromechanical modelling of alumina trihydrate filled poly (methyl methacrylate) composites. Int J Mater Struct Integr 7:31–47CrossRefGoogle Scholar
- Teng H (2010) Stiffness properties of particulate composites containing debonded particles. Int J Solids Struct 47:2191–2200CrossRefGoogle Scholar
- Tijssens MG, Sluys BL, van der Giessen E (2000) Numerical simulation of quasi-brittle fracture using damaging cohesive surfaces. Eur J Mech A/Solids 19:761–779CrossRefGoogle Scholar
- Vendroux G, Knauss W (1998) Submicron deformation field measurements: part 2 Improved digital image correlation. Exp Mech 38:86–92CrossRefGoogle Scholar
- Wang X, Wang L, Su Q, Zheng J (2013) Use of unmodified SiO\(_2\) as nanofiller to improve mechanical properties of polymer-based nanocomposites. Compos Sci Technol 89:52–56CrossRefGoogle Scholar
- Weng G (1992) Explicit evaluation of Willis’ bounds with ellipsoidal inclusions. Int J Eng Sci 30:83–92CrossRefGoogle Scholar
- Williams J (2010) Particle toughening of polymers by plastic void growth. Compos Sci Technol 70:885–891CrossRefGoogle Scholar
- Wypych G (2016) Handbook of fillers. Elsevier, AmsterdamGoogle Scholar
- Xu X-P, Needleman A (1993) Void nucleation by inclusion debonding in a crystal matrix. Model Simul Mater Sci Eng 1:111CrossRefGoogle Scholar
- Young RJ, Beaumont PWR (1977) Failure of brittle polymers by slow crack growth. J Mater Sci 12:684–692. https://doi.org/10.1007/bf00548158 CrossRefGoogle Scholar
- Zhu Z-K, Yang Y, Yin J, Qi Z-N (1999) Preparation and properties of organosoluble polyimide/silica hybrid materials by sol–gel process. J Appl Polym Sci 73:2977–2984. https://doi.org/10.1002/(SICI)1097-4628(19990929)73:14%3c2977::AID-APP22%3e3.0.CO;2-J CrossRefGoogle Scholar

## Copyright information

**Open Access**This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.